**Stability and crystal structures of iron carbides: A comparison between the semi-empirical modified**

**embedded atom method and quantum-mechanical DFT calculations**

C. M. Fang,1,2,*M. A. van Huis,1,3B. J. Thijsse,4and H. W. Zandbergen2

1_{Materials Innovation Institute (M2I), Mekelweg 2, 2628 CD Delft, The Netherlands}

2* _{Kavli Institute of Nanoscience, Delft University of Technology, Lorentzweg 1, 2628 CJ Delft, The Netherlands}*
3

_{EMAT, University of Antwerp, Groenenborgerlaan 171, 2020 Antwerp, Belgium}4_{Department of Materials Science and Engineering, Delft University of Technology, Mekelweg 2, 2628 CD Delft, The Netherlands}

(Received 7 November 2011; published 29 February 2012)

Iron carbides play a crucial role in steel manufacturing and processing and to a large extent determine the physical properties of steel products. The modified embedded atom method (MEAM) in combination with Lee’s Fe-C potential is a good candidate for molecular dynamics simulations on larger Fe-C systems. Here, we investigate the stability and crystal structures of pure iron and binary iron carbides using MEAM and compare them with the experimental data and quantum-mechanical density functional theory calculations. The analysis shows that the Fe-C potential gives reasonable results for the relative stability of iron and iron carbides. The performance of MEAM for the prediction of the potential energy and the calculated lattice parameters at elevated temperature for pure iron phases and cementite are investigated as well. The conclusion is that Lee’s MEAM Fe-C potential provides a promising basis for further molecular dynamics simulations of Fe-C alloys and steels at lower temperatures (up to 800 K).

DOI:10.1103/PhysRevB.85.054116 *PACS number(s): 75.50.Bb, 64.60.My, 71.15.Nc, 61.50.Lt*

**I. INTRODUCTION**

Carbon exists in steels as interstitial atoms in ferrite,
austenite, and martensite phases. It is also present in iron
carbide phases, as precipitates in a ferrite matrix or in
pearlite-type or bainite-pearlite-type microstructures.1–4 _{The iron carbides are}
of crucial importance in the design of the material properties
of steels and Fe alloys.1–6 _{Good examples are the so-called}
transformation-induced plasticity (TRIP) steels that are a
promising group of cold formable steels that combine a very
high ductility with high strength.7–9_{The TRIP steels are now}
used in a few applications in the body in white of European
and Japanese automobile industry.9,10 _{By means of }
scan-ning electron microscopy (SEM) and transmission electron
microscopy (TEM), many investigations were performed on
the phase characterization and the related microstructures of
industrial TRIP and TRIP-assisted multiphase steels.7–14 _{In}
addition, computational simulations have proven to be very
useful for investigation of FeC phases in steels. Parameter-free
first-principles approaches have been employed, but they
were applied only to small systems due to the computational
limits.15–22 _{For large systems, atomistic simulation methods,}
such as the pair-potential approach (PPA),23,24 _{the embedded}
atomic method (EAM),25–31_{and the recently adopted modified}
embedded atom method (MEAM),32–34 are very valid. The
main uncertainty in the large-scale simulations is the model
describing interactions between atoms.35 _{Recently, Lee }
pub-lished a new Fe-C potential within the MEAM formalism.36
This new Fe-C potential has been applied for pure iron,
inter-stitial C in Fe, as well as several iron carbides.37–40_{However,}
there is no systematic investigation of the applicability of Lee’s
MEAM potential to iron carbides,36–40 _{which play a crucial}
role in steel manufacturing and processing. In this paper, we
summarize our recent work in pure iron and iron carbides
phases using the MEAM approach. A comparison of the
MEAM calculations with the first-principles density functional

theory (DFT) within the generalized gradient approximation (GGA) and the conventional local density approximation (LDA) approaches, as well as with the available experimental values in literature, is presented. These results are helpful for understanding the relative stability of iron and iron carbides and, in particular, for sensible analysis of large-scale molecular dynamics simulations of Fe and Fe-C systems.

**II. CALCULATION DETAILS**
**A. Formation energies**

*The formation energy (E) of an iron carbide (Fe*nCm)

*from the pure solids of the elements (α phase and graphite)*
can be described as:

*E= E(Fe*_{n}Cm)*− [nE(Fe) + mE(C)].* (1)

To assess the relative stability of different iron carbides, we
*use the formation energy per atom (Ef*):

*Ef* *= E/(n + m).* (2)

*The energy EC*to insert C in Fe sublattices to form FenC is

defined as:

*EC* *= E(Fe*nC)*− [nE(Fe) + E(C)].* (3)

*Positive values of EC* *(Ef*) indicate that the Fe
sub-lattices with interstital C atoms or the iron carbides are
metastable, while negative values indicate genuine stability
of the systems, relative to the elemental solids (ferrite and
graphite). At a temperature of 0 K and a pressure of 0 Pa, the
enthalpy difference is equal to the energy difference, that is
*H*(FenCm)*= E(Fe*nCm), when we ignore the zero-point

**B. Lee’s Fe-C MEAM potential**

In 2006, Lee published his work on the MEAM potential
for the Fe-C system, including the effects of second nearest
neighbors.36_{In the MEAM, the total energy of an Fe-C system}
is given in the following form:

*E*=
i
*Fi(ρi)*+1*/*2
*i*
*j*
*φij(Rij),* (4)

*where Fi(ρi) is the embedding function for an atom i *
*embed-ded in a background electron density ρi, and φij(Rij*) is the pair
*potential for the interaction between atoms i and j separated*
*by a distance of Rij*. The background electron density at each
atomic site is computed by combining several partial electron
density terms for different angular contributions with weight
factors. In the Lee MEAM potentials, the second nearest
neighbors interactions were taken into account by adjusting
the screening parameters. Details of the MEAM formalism
and the parameters for the Fe-C system were described in
Refs.33–36.

Lee’s potential has been integrated into the molecular
dynamics codeCAMELION,31,41which was used in this work.
All simulations have been performed using a barostat and
a thermostat of the Berendsen type.42 _{Unless mentioned}
otherwise, results are given for 0 K (after rapid cooling)
and 0 bar. During energy minimization, the relative atomic
positions were left unconstrained in the unit cells for the binary
iron carbide phases, except for the simple structures, such as
NaCl-type, CsCl-type, and ZnS-type structures of FeC, where
the formation energies and lattice parameters were obtained
by their energy-volume relationships.

**C. DFT calculations**

All the DFT calculations were carried out using the
*first-principles’ Vienna ab initio Simulation Program (VASP)*43–45
employing density functional theory (DFT) within the
projector-augmented wave (PAW) method.46,47_{Both the }
spin-polarized GGA formulated by Perdew, Burke, and Ernzerhof
(PBE)48 and the conventional spin-polarized LDA49 were
employed for the exchange and correlation energy terms. The
cutoff energy of the wave functions was 500.0 eV. The cutoff
energy of the augmentation functions was about 644.8 eV. The
electronic wave functions were sampled on dense grids, e.g.

a 12*× 12 × 12 grid with 84 k points or a 24 × 24 × 24*
*grid with 364 k points in the irreducible Brillouin zone (BZ)*
*of θ -Fe*3*C or of α-Fe, respectively, using the Monkhorst and*

Pack method.50 _{Structural optimizations were performed for}
both lattice parameters and coordinates of atoms. The tests
*of k-mesh and cutoff energies showed a good convergence*
*(<1 meV/atom).*

**III. RESULTS**

**A. Classification of iron carbides**

*There are four solid phases for pure iron: ferrite or α-Fe*
(bcc), which is the ground state at ambient conditions; austenite
*or γ -Fe (fcc), which is stable in the temperature range between*
*1185 to 1667 K; the high-temperature phase δ-Fe (bcc)*
(stable from 1667 K to the melting point 1811 K); and the
*high-pressure phase ε-Fe (hcp). The δ-Fe phase is isostructural*
*with α-Fe (bcc). Their difference lies in magnetism: the*
*ground state of α-Fe (bcc) is ferromagnetic (FM) while δ-Fe*
(bcc) is nonmagnetic (NM).51 _{Table} _{I} _{shows the MEAM}
results for bcc-Fe and fcc-Fe compared with those calculated
with DFT-LDA and DFT-GGA. As expected, the MEAM
lattice parameters and formation energies reproduce the former
MEAM calculations.36 The DFT-GGA correctly predicts that
the FM bcc-Fe phase is the ground state, while the DFT-LDA
predicts the wrong ground state [nonmagnetic, (NM-)Fcc].
The MEAM lattice parameters agree with the experimental
values much better than those from DFT-GGA and DFT-LDA.
For bcc-Fe, this was to be expected because the MEAM
potential was explicitly fitted to the lattice parameter. All three
computational methods confirm that the ground state of iron
*is the ferrite phase, while the γ - and ε-Fe (not shown) phases*
are less stable (TableI). That agrees with former DFT-GGA
calculations.51–56

There are several phases for C, and at ambient conditions,
the stable phase is graphite. However, it is difficult to
perform MEAM calculations for graphite due to the interlayer
Van der Waals interaction, which is not included in the
MEAM potential. Experiments showed that graphite is about
*17 meV/C more stable than the diamond phase.*18,57Therefore,
the MEAM energy for graphite is obtained from that of the
diamond phase after this correction. The calculated lattice
*parameter for diamond is a* = 3.558 ˚A, in agreement with
the experimental value.

TABLE I. Calculated results for the iron phases using Lee’s Fe-C MEAM potential compared with the DFT-GGA and DFT-LDA calculations as well as with the experimental values. The deviations (%) of the calculated lattice parameters from the experimental values are included (FM= ferromagnetic, NM = nonmagnetic).

bcc Fe fcc Fe
MEAM
Lattice parameters ( ˚A) *a*= 2.864 (−0.1%) *a*= 3.604 (+0.5%)
*EeV/Fe* 0.0 0.062
DFT-LDA
Lattice parameters ( ˚A) *a*= 2.751 (−4.0%) *a*= 3.372 (−6.3%)
*EeV/Fe* 0.0 (FM) −0.066 (NM)
DFT-GGA
Lattice parameters ( ˚A) *a*= 2.833 (−0.9%) *a*= 3.477 (−3.1%)
*EeV/Fe* 0.0 (FM) 0.060 (NM)

TABLE II. Calculated lattice parameters at 0 K using Lee’s Fe-C potential within the MEAM approach compared with the DFT-GGA and DFT-LDA methods and compared with experimental values (Tetra= tetragonal, Orth = orthorhombic).

MEAM lattice DFT-GGA lattice DFT-LDA lattice Experimental lattice Formula Lattice parameters ( ˚A) parameters ( ˚A) parameters ( ˚A) parameters ( ˚A) bcc based

*α*-Fe16C Tetra *a* *= 5.616* *a* *= 5.6382* *a* *= 5.457*

*c* *= 6.228* *c* *= 6.0757* *c* *= 5.875*

*c/a* *= 1.109* *c/a* *= 1.078* *c/a* *= 1.076*

*α*-Fe16C2 Tetra *a* *= 5.697* *a* *= 5.6553* *a* *= 5.4721*

*c* *= 6.309* *c* *= 6.2624* *c* *= 6.1182*

*c/a* *= 1.109* *c/a* *= 1.107* *c/a* *= 1.118*

*α*-Fe3C2 Orth *a* *= 5.464* *a* *= 5.471* *a* *= 5.428*
*b* *= 3.189* *b* *= 2.747* *b* *= 2.688*
*c* *= 10.518* *c* *= 11.202* *c* *= 10.805*
fcc based
*γ*-FeC (NaCl-) fcc *a* *= 4.096* *a* *= 4.001* *a* *= 3.923*
*γ*-FeC (CsCl-) fcc *a* *= 4.096* *a* *= 4.001* *a* *= 3.923*
*γ*-FeC (ZnS-) fcc *a* *= 4.325* *a* *= 4.2541* *a* *= 4.1775*
*γ*-Fe4C Cubic *a* *= 3.923(+1.2%)* *a* *= 3.767(−2.8%)* *a* *= 3.643(−6.4%)* *a* *= 3.875*
*γ*-Fe8C Cubic *a* *= 7.403(1.1%)* *a* *= 7.247(−1.0%)* *a* *= 6.957(−5.0%)* *a* *= 7.323*
hcp family
*θ*-Fe3C Orth *a* *= 5.165(+1.0%)* *a* *= 5.037(−0.9%)* *a* *= 4.841(−6.7%)* *a* *= 5.082*
*b* *= 6.277(−5.5%)* *b* *= 6.720(−0.2%)* *b* *= 6.516(−3.2%)* *b* *= 6.733*
*c* *= 4.674(+3.0%)* *c* *= 4.482(−0.3%)* *c* *= 4.329(−4.1%)* *c* *= 4.514*
o-Fe7C3 Orth *a* *= 4.851(+6.9%)* *a* *= 4.517(−0.5%)* *a* *= 4.396(−3.2%)* *a* *= 4.540*
*b* *= 6.684(−2.8%)* *b* *= 6.856(−0.3%)* *b* *= 6.669(−3.1%)* *a* *= 6.879*
*c* *= 11.447(−4.1%)* *c* *= 11.733(−1.7%)* *c* *= 11.409(−4.4%)* *c* *= 11.940*
*η*-Fe2C Orth *a* *= 4.342(−7.7%)* *a* *= 4.707(+0.1%)* *a* *= 4.245(−9.8%)* *a* *= 4.704*
*b* *= 4.419(+2.9%)* *b* *= 4.280(0.3%)* *b* *= 4.356(+1.4%)* *b* *= 4.295*
*c* *= 2.854(+0.8%)* *c* *= 2.824(−0.2%)* *c* *= 2.794(−1.3%)* *c* *= 2.830*
*ζ*-Fe2C Orth *a* *= 4.280* *a* *= 4.2997* *a* *= 4.255*
Pbcn *b* *= 5.456* *b* *= 5.4810* *b* *= 5.293*
*c* *= 4.829* *c* *= 4.8511* *c* *= 4.693*

Table II lists structural information of important iron
carbides in steels,4,18–21 _{according to MEAM and DFT }
cal-culations and experimental data. These iron carbides include
three different types according to their Fe sublattices.4,58,59
*The bcc family contains the so far unanalyzed α*-Fe16C,

*α*-Fe16C2*, and α*-Fe3C2 phases [see Figs. 1(a) and 1(b)],

which consist of bcc- Fe sublattices with C interstitial atoms
occupying the octahedral sites. The second type is the fcc
*family, of which the structures are based on the γ -Fe sublattice*
with C at the octahedral or tetrahedral sites [Figs.1(c) and

1(d)*]. The third is the ε-family [Figs.* 1(e) and 1(f)] with
*members η-Fe*2*C and θ -Fe*3C, which play important roles in

manufacturing processes, as well as in the microstructures and physical properties of Fe-C steels. Details of the results will be discussed in Subsec. C.

**B. Formation energies of iron carbides**

Figure 2 shows the formation energies obtained from the calculations. There are few experimental values of high accuracy due to the difficulties associated with the preparation of homogeneous samples. Overall, the DFT-GGA results agree best with the experimental values, while the DFT-LDA overestimates the stability. The MEAM results are in between. Below, we discuss the calculation results in detail.

*In the martensite phase, as shown by Domain et al., C atoms*
occupy the octahedral sites.4,56,58 _{The MEAM calculations}
*show that for dilute C in α-Fe, the C solution energy is*
*1.17 eV/C, in good agreement with Lee’s calculations.*36_{}
Fig-ure1*shows the schematic structures for α*-Fe16*C, α*-Fe16C2

[both in Fig.1(a)*], and α*-Fe3C2 [Fig.1(b)]. The calculated

*formation energy for α*-Fe16C phase by the MEAM approach

*is 0.92 eV/C, which is smaller than the solution energy of*
*dilute C in ferrite (1.17 eV/C). This value, 0.92 eV/C, is*
about twice the value found using the DFT-GGA approach
*(0.45 eV/C). However, it is close to the value (0.89 eV/C) from*
the DFT-LDA calculations. Please note that the experimental
values for dilute C in ferrite have a scattering range (from
about 0.4 to 1.2 eV).36,56The MEAM calculations showed for
*α*-Fe16C2*the formation energy is lowered to about 0.81 eV/C*

*from 0.92 eV/C (for α*-Fe16C), with the same trend for DFT, as

shown in Fig.2. The phase of the highest carbon concentration,
*α*-Fe3C2, is calculated to be slightly favored with respect

to the elemental solids (ferrite and graphite) by the MEAM
*approach. The DFT-GGA calculations show that α*-Fe3C2

*is metastable with a formation energy of 135 meV/atom.*
However, the MEAM result for this carbide is not far
*from the DFT-LDA result, about 4 meV/atom difference*
(Fig.2).

(a) (b)

(c) (d)

(e)

(f)

FIG. 1. (Color online) Schematic structures of the iron carbides
*from the bcc family: (a) α*-Fe16*C, α*-Fe16C2 *and (b) α*-Fe3C2;

*from the fcc family: (c) γ*-FeC with NaCl-type structure and (d)

*γ*-Fe4*C; from the hcp family: (e) the cementite phase θ -Fe*3C and

*(f) the H¨agg phase η-Fe*2C. The small black spheres represent Fe

atoms, big green/medium gray spheres C atoms. The blue/light gray
*spheres in (a) represent another occupied C site to form α*-Fe16C2.

*In (c) the small black and the green/gray spheres in the γ*-Fe4C

structure indicate the 4 Fe and 1 C atom positions, respectively. In the
FeC structure, again, blue (light gray)/green (medium gray) spheres
indicate C atoms and black spheres Fe atoms. Lattice parameters
*(a,b,c) are indicated in panels (b), (e), and (f).*

*For the fcc family, we start from γ*-FeC, having the
NaCl-type structure [Fig. 1(c)]. The calculated (MEAM)
*formation energy is 405 meV/atom, which is much smaller*
than the GGA result. However, this value is close to the
*LDA results (415 meV/atom), as shown in Fig.* 2. All

0 0.1 0.2 0.3 0.4 0.5 C concentration -0.4 -0.2 0 0.2 0.4 0.6 0.8

Formation energy (eV/atom)

ZnS-

CsCl-

NaCl-ζ− η−

FIG. 2. (Color online) The calculated formation energies for the
iron carbides using different approaches. The crystal structures are
displayed in Fig. 1, the calculated lattice parameters are listed in
TableII. The different colors represent the calculated results by means
of MEAM (green/light gray), DFT-GGA (red/dark gray), DFT-LDA
(blue/medium gray) and experimental values (black).61 _{The filled}

spheres represent for the bcc family, filled squares the fcc family, and filled diamonds the hcp family (see TableII).

*calculations for γ*-Fe4C give positive formation energies.

*For γ*-Fe8*C, the MEAM formation energy is 85 meV/atom,*

*close to that by DFT-GGA (110 meV/atom). In contrast, the*
*DFT-LDA predicts this phase as being too stable (Ef* =
*−40 meV/atom), considering that this phase has never been*
observed experimentally.

*The members of the hcp family, such as θ -Fe*3C (the

*cementite phase) and η-Fe*2C (the H¨agg phase) [Fig.1(e)–1(f)],

play a crucial role in the steel manufacturing processes.1–5,20
As shown in Fig. 2, the MEAM calculations show that
the order of stability for the most important hcp phases is
*(from high stability to lower): η-Fe*2*C > o-Fe*7C3*> θ*-Fe3C,

the same order as the experimental order. Meanwhile, DFT-GGA showed that in the three hcp phases, o-Fe7C3 is the

least stable, while DFT-LDA calculations show that o-Fe7C3

has the lowest formation energy. Our MEAM calculations give a moderate stability (∼−15 meV/atom) for θ-Fe3C,

the cementite phase (Fig. 2). The DFT-LDA calculations produce an even higher stability (−84 meV/atom) for θ-Fe3C

*cementite. The MEAM calculations show that η-Fe*2C is

*more stable than ζ -Fe*2C. This agrees with the DFT-GGA

calculations, as well as with the experimental observation
*that η-Fe*2C occurs frequently in tempering of quenched Fe-C

*steels, while the ζ -phase has never been observed. Please*
*note that both η-Fe*2*C and ζ -Fe*2C have similar Fe sublattices.

The major difference is the ordering of C atoms.4,19,20,59 _{In}
*η*-Fe2*C, along the c axis the carbon atoms form C-C bonds*

with lengths of about 2.8 ˚*A, while in ζ -Fe*2C, the C atoms

form zigzagged chains with longer C-C bond lengths.4,20 Meanwhile, the DFT-LDA calculations also predict wrong formation energies for all the hcp iron carbides as shown in Fig.2.

**C. Lattice parameters of iron carbides**

From TableII, we see that the MEAM lattice parameters
*of the three novel members of the bcc family (α**, α**, α*) are
in good agreement with the DFT-GGA calculations. However,
*the calculated c/a ratio (1.11) of α*-Fe16C using the MEAM

*method is almost the same as that of α*-Fe16C2, whereas the

*c/a*ratio of Fe16*C (1.08) increases to 1.11 for α*-Fe16C2using

the DFT methods.

*For γ*-FeC with the NaCl-type structure [Fig. 1(c)], the
calculated lattice parameter is 4.10 ˚A, in agreement with Lee’s
calculations.36 _{Our calculated lattice parameter is slightly}
larger than the GGA (4.00 ˚A) and LDA (3.92 ˚A) results.

*For γ*-Fe4*C and γ*-Fe8C, the MEAM calculations

repro-duce the experimental lattice parameters well, within 1.2% (TableII). In comparison, the DFT-GGA underestimates the experimental values by about 3%, and the DFT-LDA by about 6.0%.

For the well-known hcp family members, the MEAM
cal-culations give significant deviations of the lattice parameters
*from the experimental values, particularly for the b axis in*
*θ*-Fe3*C, the a axis in o-Fe*7C3*, and η-Fe*2C deviation about

+7%. Comparatively, the lattice parameters from the
DFT-GGA calculations agree well with the experimental values
(within 1.7%). The DFT-LDA calculations, however, provide
even worse agreements with the experimental values. The most
*significant one is the a axis of η-Fe*2C (the deviation is close

to 10%) using the DFT-LDA approach.

In conclusion, the MEAM approach predicts the lattice parameters of the bcc family and fcc family members well, but for the hcp family members, there are significant deviations, possibly due to the anisotropy of layered Fe hcp sublattices.

**D. Temperature dependence of iron phases and cementite**
One advantage of the semi-empirical MEAM approach
compared to DFT calculations is its ability to perform
large-scale molecular dynamics simulations. To investigate the
performance of the potentials as a function of temperature,
ferrite and austenite were used as test systems. Calculations
were performed for a cell of 16 000 bcc Fe atoms and 16 384
fcc Fe atoms. The systems were heated step by step with a step
dwell time of about 15 fs. The calculated results are shown in
Fig.3.

Disregarding entropy effects, we see that bcc Fe is more stable than fcc Fe over the whole temperature range where the systems are crystalline. The melting temperature obtained in this way is about 2200 K for bcc Fe. This is slightly higher than the experimental value (1811 K). To investigate the melting temperature of bcc Fe with more precision, additional molecular dynamics simulations were conducted. First, a large system containing about 50 000 Fe atoms is divided into two parts by connecting one half of the atoms to anchor points fixed in space and leaving the other half free. Next, the system is heated to 3000 K, as a result of which the free part melts and forms a liquid. After about 100 fs, the constraints on the other half were released, and the two parts were allowed to continue adiabatically. In this phase, a thermal equilibrium is gradually reached, with a coexistence of bcc and liquid Fe. In this way, the melting temperature of bcc Fe was obtained to be 1900 (±80) K, close to the experimental value (1811 K).

0 500 1000 1500 2000 2500 3000 Temperature (K) -4.3 -4.2 -4.1 -4 -3.9 -3.8 Potential (eV/Fe) Bcc-Fe Fcc-Fe

FIG. 3. The dependence of the calculated MEAM potential
*energy (eV/Fe) on temperature for bcc Fe and fcc Fe.*

From Fig.3, it is clear that there is no austenite window.
The austenite window (1185 to 1667 K) comes from the
Curie–Weiss magnetism disordering effects of ferrite and
austenite,51,59 _{while the MEAM potential does not take}
into account any magnetic (ordering) effects. Nonetheless,
the present calculations show that the MEAM approach is
capable of describing the relative stability of austenite in the
temperature range 0–800 K. This justifies the use of the MEAM
potential in investigations of the stability of austenite and other
phases in the treatment processes of many Fe-C steels.

*The cementite phase, θ -Fe*3C plays an important role in the

tempering of steels, and it is has a pivotal role in many
mi-crostructures, such as pearlite and bainite in steels. Knowledge
about thermal behavior of cementite is important to assess
the reliability of molecular simulations.60 _{The simulations}
*show that θ -Fe*3C remains crystalline up to a temperature of

about 750 K. The MEAM potential energy increases with
temperature, being similar to that of iron phases. The MEAM
lattice parameters of the orthorhombic cell increase with
temperature, as well. In the temperature range from about 200
to 500 K, the calculated linear thermal expansion parameters
show a slight anisotropy: 1.4× 10−5 *(1/K) for the a axis,*
and 1.2× 10−5 *(1/K) for the b and c axes. In 2004, Wood*
made careful measurements of thermal expansion parameters
*for θ -Fe*3C.61*They observed anisotropy of the a axis from the*

*band c axes, which is in line with our MEAM calculations,*
on one hand. They also observed strong impacts of magnetic
ordering: the volume expansion is about 1.8 × 10−5 *(1/K)*
*when T < T c (T c*= 480 K, the Curie temperature) and about
4,1× 10−5*(1/K) when T > T c.*61

**IV. CONCLUSIONS**

We used Lee’s Fe-C MEAM potential to investigate the relative stability and structural properties of pure iron phases and iron carbides. This MEAM potential performed well in describing the lattice parameters and cohesive energies of ferrite and austenite, as well as the lattice parameters of most Fe-C systems. Exceptions are the very high stabilities of the iron carbides having very high C concentrations such

*as α*-Fe3C2, o-Fe7C3*, and η-Fe*2*C, γ*-FeC (ZnS-type). The

accuracy of the MEAM approach is at the same level as the conventional DFT-LDA approach, in particular for steels having low C concentrations. This is a good achievement for a non-quantum mechanical approach. From the present results, it can be concluded that Lee’s MEAM potential can be applied with reasonable accuracy in molecular dynamics simulations of ferrite-austenite interfaces as well as for C in

ferrite-austenite based systems, in particular in the temperature range up to 800 K.

**ACKNOWLEDGMENTS**

This research was carried out under Project No. MC5.06280 in the framework of the Research Program of the Materials Innovation Institute M2i (www.m2i.nl), The Netherlands.

*_{Dr. Changming Fang, Kavli Institute of Nanoscience, Delft }

Univer-sity of Technology, Lorentzweg 1, 2628 CJ Delft, The Netherlands; c.fang@tudelft.nl

1_{L. J. Hofer and E. M. Cohn,}** _{Nature 167, 977 (1951).}**
2

_{D. H. Jack and K. H. Jack,}

**3**

_{Mater. Sci. Engin. 11, 1 (1973).}**4**

_{H. J. Goldschmidt, J. Iron Steel Inst. 160A, 345 (1948).}**5**

_{S. Nagakura and S. Oketani, Transactions ISIJ 8, 265 (1968).}

_{JW Christian, The Theory of Transformation in Metals and}*Alloys (Pergamon Press, Amsterdam/Boston/London/NewYork/*

Oxford/Paris/SanDiego/SanFrancisco/Singapore/Sydney/Tokyo, 2002).

6_{M. Taneike, F. Abe, and K. Sawada,}** _{Nature 424, 294 (2003).}**
7

_{S. O. Kruijver, L. Zhao, J. Sietsma, S. E. Offerman, N. H. van Dijk,}

E. M. Lauridsen, L. Margulies, S. Grigull, H. F. Poulsen, and N. H.
van Dijk,**J. Phys. IV France 104, 499 (2003).**

8_{S. van der Zwaag and J. Wang,}** _{Scr. Mater. 47, 169 (2002).}**
9

_{V. Andrade-Carozzo and P. J. Jacques,}

_{Mater. Sci. Forum 500-501,}445 (2005).

10_{O. Mur´ansky, P. ˇSittner, Zrn´ık, and E. C. Oliver,}** _{Acta Mater. 56,}**
3367 (2008).

11_{E. Jimmenez-Melero, N. H. van Dijk, L. Zhao, J. Sietsma, S. E.}

Offerman, J. P. Wright, and S. van der Zwaag,**Acta Mater. 55, 6713**
(2007).

12_{G. K. Tirumalasetty, M. A. van Huis, C. M. Fang, F. D. Tichelaar,}

Q. Xu, D. N. Hanlon, J. Sietsema, and H. W. Zandbergen,Acta
**Mater. 59, 7406 (2011).**

13_{H. Letner, M. Bishof, H. Clemens, S. Erlach, B. Sonderegger,}

E. Kozeschnik, J. Svoboda, and F. D. Fischer,Adv. Engin. Mater.
**8, 1066 (2006).**

14_{K. H. Lo, C. H. Shek, and J. K. L. Lai,}** _{Mater. Sci. Engin. R 65, 39}**
(2009).

15_{IR Shein, NI Medvedeva, and AL Ivanovskii,}** _{Physica B 371, 126}**
(2006).

16_{HI Faraoun, YD Zhang, C Esling, and H Aourag,}** _{J. Appl. Phys. 99,}**
093508 (2006).

17_{M. H. F. Sluiter, Phase Stability of carbides and Nitrides in Steel,}

Mat. Res. Soc. Proc. Vol. 979 E., edited by D. N. Seidman, P. Bellon, C. Abromeit, and J. L. Boquet, MRS Fall-meeting Boston 2006, session HH(200), paper number: 0979-HH14-03.

18_{C. M. Fang, M. A. van Huis, and H. W. Zandbergen,}_{Phys. Rev. B}
**80, 224108 (2009).**

19_{C. M. Fang, M. A. van Huis, M. H. F. Sluiter, and H. W. Zandbergen,}
**Acta Mater. 58, 2968 (2010).**

20_{C. M. Fang, M. A. van Huis, and H. W. Zandbergen,}** _{Scr. Mater. 63,}**
618 (2010).

21_{Z. Q. Lv, S. H. Sun, P. Jiang, B. Z. Wang, and W. T. Fu,}_{Comput.}
**Mat. Sci. 42, 692 (2008).**

22_{J. H. Jang, I. G. Kim, and H. K. D. H. Bhadeshia,}** _{Scr. Mater. 63,}**
121 (2010).

23_{J. Y. Xie, N. X. Chen, J. Shen, L. D. Teng, and S. Seetharaman,}
**Acta Mater. 53, 2727 (2005).**

24_{K. O. E. Henriksson and K. Nordlund,}** _{Phys. Rev. B 79, 144107}**
(2009).

25_{M. S. Daw and M. I. Baskes,}** _{Phys. Rev. Lett. 50, 1285 (1983).}**
26

_{M. S. Daw and M. I. Baskes,}

**27**

_{Phys. Rev. B 29, 6443 (1984).}_{M. Ruda, D. Farkas, and G. Garcia,}

_{Comput. Mater. Sci. 45, 550}(2009).

28_{M. I. Mendelev, S. Han, D. J. Srolovitz, G. J. Ackland, D. Y. Sun,}

and M. Asta,**Philos. Mag. 83, 3977 (2003).**

29_{D. J. Hepburn and G. J. Ackland,} ** _{Phys. Rev. B 78, 165115}**
(2008).

30_{Q. F. Fang and R. Wang,}_{Phys. Rev. B 62, 9317 (2000).}

31_{C. Bos, J. Sietsma, and B. J. Thijsse,}** _{Phys. Rev. B 73, 104117}**
(2006).

32_{M. I. Baskes,}_{Phys. Rev. B 46, 2727 (1992).}

33_{B. J. Lee and M. I. Baskes,}** _{Phys. Rev. B 62, 8564 (2000).}**
34

_{B. J. Lee, J. H. Shim, and M. I. Baskes,}

_{Phys. Rev. B 68, 144112}(2003).

35_{K. Nordlund and S. L. Dudarev,}** _{C. R. Physique 9, 343 (2008).}**
36

_{B. J. Lee,}

_{Acta Mater. 54, 701 (2006).}37_{B. J. Lee, T. H. Lee, and S. J. Kim,}** _{Acta Mater. 54, 4597 (2006).}**
38

_{H. K. Kim, W. S. Jung, and B. J. Lee,}

**39**

_{Acta Mater. 57, 3140 (2009).}_{B. J. Lee,}

_{JPEDAV 30, 509 (2009).}40_{J. W. Jang, J. Kwon, and B. J. Lee,}** _{Scr. Mater. 63, 39 (2010).}**
41

_{B. J. Thijsse, “Doing Molecular Dynamics with}

_{CAMELION}

_{,”}

*Virtual Materials Lab, Department of Materials Science and*
*Engineering, Delft University of Technology, The Netherlands,*

[http://web.mac.com/barend.thijsse].

42_{H. J. C. Berendsen, J. P. M. Postma, W. F. van Gunstere, A. Dinola,}

and J. R. Haak,**J. Chem. Phys. 81, 3684 (1984).**
43_{G. Kresse and J. Hafner,}** _{Phys. Rev. B 47, 558 (1993).}**
44

_{G. Kresse and J. Hafner,}

**45**

_{Phys. Rev. B 49, 14251 (1994).}_{G. Kresse and J. Furthm¨uller,}

**46**

_{Comput. Mat. Sci. 6, 15 (1996).}_{P. E. Bl¨ochl,}

_{Phys. Rev. B 50, 17953 (1994).}47_{G. Kresse and J. Furthm¨uller,}** _{Phys. Rev. B 59, 1758 (1999).}**
48

_{J. P. Perdew, K. Burke, and M. Ernzerhof,}

_{Phys. Rev. Lett. 77, 3865}(1996).

49_{D. M. Ceperley and B. J. Alder,}** _{Phys. Rev. Lett. 45, 566 (1980).}**
50

_{H. J. Monkhorst and J. D. Pack,}

**51**

_{Phys. Rev. B 13, 5188 (1976).}_{C. Zener,}

_{J. Appl. Phys. 22, 372 (1955).}52_{H. C. Herper, E. Hoffmann, and P. Entel,}** _{Phys. Rev. B 60, 3839}**
(1999).

53_{D. W. Boukhvalov, Yu. N. Gornostyrev, M. I. Katsnelson, and A. I.}

54_{M. van Schilfgaarde, I. A. Abrikosov, and B. Johansson,}_{Nature}
**(London) 400, 46 (1999).**

55_{C. Amador, W. R. L. Lambrecht, and B. Segall,}** _{Phys. Rev. B 46,}**
1870 (1992).

56_{C. Domain and C. S. Becquart,} ** _{Phys. Rev. B 65, 024103}**
(2001).

57_{GTE Unary Database version v4.4, 20 July 2001, see e.g. Elements}

*and binary systems from Ag–Al to Au to Tl, in Thermodynamic*
*Properties of Inorganic Materials, edited by P. Franke and*

D. Neusch¨ultz, Landolt-B¨ornstein: New Series Group 4: Phys.

Chem. Vol 19 XXVI, Scientific Group Thermodata Europe (SGTE), (Springer, Berlin, 2002).

58_{C. Domain, C. S. Becquart, and J. Foct,}** _{Phys. Rev. B 69, 144112}**
(2004).

59_{C. M. Fang, M. H. F. Sluiter, M. A. van Huis, C. K. Ande, and}

H. W. Zandbergen,**Phys. Rev. Lett. 105, 055503 (2010).**

60_{M. Umemoto, Z. G. Liu, K. Matsuyama, and K. Tsuchiya,} _{Scr.}
**Mater. 45, 391 (2001).**

61_{I. G. Wood, L. Voc¨Iadlo, K. S. Knight, D. P. Dobson, W. G. Marshall,}